Presentation on theme: "No. 3 of 20 Testing of Geosynthetics by Prof. Dr.-Ing. Müller-Rochholz Fachhochschule Münster and tBU - Institut für textile Bau-und Umwelttechnik GmbH,"— Presentation transcript:
No. 3 of 20 Testing of Geosynthetics by Prof. Dr.-Ing. Müller-Rochholz Fachhochschule Münster and tBU - Institut für textile Bau-und Umwelttechnik GmbH, Greven The information presented in this document has been reviewed by the Education Committee of the International Geosynthetics Society and is believed to fairly represent the current state of practice. However, the International Geosynthetics Society does not accept any liability arising in any way from use of the information presented.
General Product Identification Polymer identification Geometrical information Thickness Grid opening size / pitch dimensions Mass per unit area
4 oven heat flow mW/mg temperature °C 6 1. controlled heating of oven specimen in pan 2. inert dummy in pan 3. heat flow sensors 4. monitor and control-PC 5. result graph 6.crystal melting point Polymer Identification
DSC- Curve of a Polypropylene Sample
Geometric Information 2 kPa Schematic 25 cm² thickness metal base
Mass / Unit Area (mua) Mass per unit area (mua) (ISO 9864; EN 965 : 1995 ASTM) the mass per unit area is one of the most often used characteristic values, giving the price creating mass of the raw material Specimens are cut preferably with a circular cutter, the number depends on the specimen size; Minimum 3, each 100 cm² to a maximum of 10 specimen, and then weighed to accuracy of g and calculate the mua. 100 cm² Balance.001 g mua = g/m²
Mechanical Properties Short-term tensile strength and dependent deformation Long-term tensile behaviour (creep/creep rupture) Long-term compressive creep behaviour (with/without Shear stress) Resistance against impact or punching Static puncture test, rapid puncture Resistance against abrasion Friction properties Direct shear, inclined plane test, pullout resistance Protection efficiency Damage during installation Geosynthetics or composites internal strength Geosynthetic reinforcement segmental retaining wall unit connection testing
Short-term tensile strength and dependent deformation (standards see table below) Mechanical Properties
Testing machine with video-extensometer Capstain clamp for geogrid with laser- extensometer Mechanical Properties
Force - Strain Behaviour of Geosynthetics
Tensile Creep and Creep Rupture EN ISO : 1996 ASTM) Tensile creep tests give information on time- dependent deformation at constant load. Creep rupture tests give time until failure at constant load. A deformation measurement is not necessary for creep rupture curves. Loads for creep testing are most often dead weights, often enlarged by lever arms.
Creep Test Rigs – set up in a controlled environment, free from vibrations
Multiple Creep Rupture Rigs in a Temperature Controlled Chamber
Creep Test Results. Creep CurvesCreep Rupture Results are plotted for creep as linear deformation vs log time For creep rupture linear or log load vs log time. Typical curves are shown
Isochronus Curves Isochronus curves From creep curves at different stress grades isochronous stress strain curves may be derived or extrapolated for calculation of structures deformation at a given time.
Compressive Behaviour (EN ISO 13432) thickness (mm) time /h) Compressive creep random wire drainage product
thickness (mm) time (h) Compressive Creep Cuspated Fin Drainage Product
time (h) Horizontal Displacement Thickness Creep Under Normal and Shear Stress - Cuspated Fin Drainage Product
Resistance To Static Puncture Static Puncture Test: The Test CBR (EN ISO : 1996) The use of soil mechanics California Bearing Ratio (CBR) apparatus for this static puncture test, has resulted in the unusual name for this test. A plunger of 50mm diameter is pushed at a speed of 50 +/- 10mm min onto and through the specimen clamped in the circular jaws. Measurement of force and displacement are taken. The test is widely used for geotextiles, it is not applicable to grids, and the test provides useful data for geomembranes.
CBR - device in testing machine Inserting specimen in hydraulic CBR- clamps
displacement mm CBR Force kN PP - tape Fabric Typical CBR-curve force vs displacement
PYRAMID PUNCTURE (ASTM ) Details of Apparatus
Dynamic Puncture Test : Cone Drop Test (ISO 13433, EN 918 : 1995) A 1kg pointed cone is dropped from a height of 1m onto a specimen, held tight in a circular clamp The diameter of a hole created is measured by means of a graduated aluminium cone scale. 1. Head, release mechanism to suit laboratory requirements 2. Guide rod 3. Cone 4. Metal screen 5. Screen 6. Clamping plates 7. Test specimen 8. Levelling screws Note:This diagram is not to scale
Measuring Cone for Cone Drop Test
Impact Resistance Test (CEN TC 189 WI 14; ISO draft) Efficiency of protection materials can be tested by dropping a hemispherical shaped weight onto a specimen placed on a lead plate on a resilient base. The impression in the lead and the condition of the specimen are recorded. Lighter round shaped drop weights are used for other geosynthetics. The deformation of a metal sheet under the tested material gives quantitative results.
Impact Resistance Test Drop weight, lead platen, specimen under ring
Layout of the Impact Test Apparatus
Impact Resistance Test (performance test : BAW) 2 m 67.5 kg Result of drop tests - no penetration A heavy drop weight (67.5 kg) is dropped from 2 m height on the geosynthetic placed on sand and fixed in a ring. The result is a penetration yes or no decision. The Test
Abrasion Resistance (EN ISO : 1995) Emery cloth of a specific grade is moved linearly along the specimen. After 750 cycles the abraded specimen is tested to measure the residual tensile strength or hydraulic properties Example of Apparatus with Sliding Block
Specimen before test Specimen after abrasion test
Force in N Strain in % PP-tape fabric: warpweft Force vs displacement of abraded specimen (lower lines) to undamaged specimen (upper line) Force in N Strain in %
Direct Shear Friction (EN ISO : 1998) Reinforcing geosynthetics develop their tensile resistance by the transfer of stresses from the soil to the fabric through friction. The friction ratio is defined as the angle of friction, the ratio of the normal stress to the shear stress. Low normal stresses may be tested by an inclined plane test and higher normal stresses by direct shear or by pull out test. Direct shear (EN ISO ) The friction partners are placed one in an upper box, the other in the lower box. The lower box is moved at a concentrate of displacement (index testing: 1 mm/min) while recording force and displacement. The results for three normal stresses (50, 100, 150 kPa) are plotted, the value of friction angle is calculated
Section Through Shearbox Test
Inclined Plane Test (EN ISO ) The friction partners to be tested (geomembrane/geosynthetic; geomembrane/soil; geosynthetic/soil) are set up on a inclinable steel table. Movement of the upper box and inclination are measured while lifting the table by 3 degrees/min. When the upper box moves 50mm the test is stopped and the angle of the table is taken as the angle of friction for the chosen materials combination. The normal stress must be recalculated for the resulting angle at the end of the test.
Inclined Plane Test: Typical Graph
Pullout Resistance (1) A strip of the geosynthetic, just narrower than the width of the box, is pulled out of a soil filled box. A load is applied to the soil geosynthetic by pneumatic, hydraulic system or deadweight system. Force and deformation are recorded for several points of the material inside the box.
Pullout Resistance (2) Force transfer at the point where the geosynthetic leaves the apparatus must be avoided. It is important to design a system at the front of the pullout box which avoids transferring load to the box. Results may be max force at rupture or slippage or plots of force v deformation.
Pullout Box Plan view and typical gauge placement Pullout resistance versus percent strain of sections of pullout specimen during test
Protection Efficiency The ability of a geotextile to protect a geomembrane is quantified by a test based on a German procedure. The deformation of a lead plate, loaded with standard M10 nuts, used as a consistently reproducible granular material. The efficiency of the geotextile to protect a geomembrane is calculated from the depth and width of the indentations.
Protection Efficiency Arrangement of Test Apparatus
Damage During Installation The CEN-ISO standard applies a cyclic load to a platen (100 x 200) pressing via a layer of Corundum aggregate placed on top of the geosynthetic being tested. (Corundum is a trade name for a sintered aluminium oxide. After 200 cycles between 5 kPa and 900 kPa maximum stress the specimen is exhumed and may be subject to a tensile test for the residual strength for reinforcement applications, or for filtration the hydraulic properties for filtration applications. A performance test requires the soil and fill to be used on the site and the equipment to spread and compact the material. Typical results of an index-test are shown
Damage During Installation (ENV ISO : 1997) The forces applied to a geosynthetic during installation can be the most severe loading that will be applied to the material, It is therefore necessary to have a test which simulates the installation process.
Plan on apparatus Filling Corundum into upper box Cyclic loading Damage During Installation
Material Before (left) and After (right) Damage Test
Geosynthetics (composites internal strength) (EN ISO ) If a failure of internal junctions may cause failure of a structure, the strength of these junctions can be tested. CEN WG 3 is developing a 3 part test. Geocells: The loading of a internal geocell-connection may be of: - a tensile shear type - a peeling type - a splitting type or of combinations.
A Typical Junction Strength Test
Hydraulic Properties Water permeability characteristics normal to plane, without load Constant head Falling head Water flow capacity in their plane Characteristic opening size
Hydraulic Properties: Water permeability characteristics normal to the plane, without load ( ENISO : 1999) When geosynthetics are working as filters, they are required to allow water through freely but soil grains need to be retained. Some very fine soil grains are allowed through such that a stable secondary filter is developed in the contact soil zone. The water flow may be determined at stationary (time independent) conditions i.e. constant flow at constant water head or at in stationary conditions, i.e. falling head.
Constant Head Test Example of apparatus for the constant head method In Darcys equation v = k v. I v = speed of flow (m/s) i = hydraulic gradient = head difference/specimen thickness De-aired water passes the specimen charged with normal stresses from top to bottom (multilayer specimen of mm are used), flow vs time is measured and expressed as a kv (kn)-factor.
Falling Head Method Examples of apparatus for the falling head method De-aired water passes the specimen charged with normal stresses from top to bottom (multilayer specimen of mm are used), flow vs time is measured and expressed as a kv (kn)-factor.
Water Flow Capacity in the Plane (EN ISO : 1999) In drainage applications water needs to flow in the plane of the geosynthetic. Tests according to EN-ISO or ASTM differ in specimen size, but use the same basic principles. 1 water supply 2 water collection 4 specimen 7 foam 8 load 9 loading platen 10 overflow weirs at hydraulic gradients 0,1 and 1,0 water reservoir base Typical Example of Apparatus
CEN - apparatus in plane flow Specimen in apparatus, net core with soft contact faces
Flow is measured at constant water head and expressed either as k H (k p ), unit m/s, or as flow capacity, unit l/s per m width of the product at given gradient. The flow value is dependent on the thickness of the product, as some products compress under load the flow values are time dependant.For a long-term design, flow values need to be corrected for the compressive creep of the product.. Typical examples of in- plane water flow capacity curves Normal compressive stress (kPa)
Characteristic Opening Size (EN ISO : 1999) To determine, which grain size can passing through a geosynthetic and which is retained, a wet sieving test is used with a standard soil. The soil passing the geotextile is extracted from the water and sieved again. A characteristic value O 90- is calculated according to EN ISO O 90 = d 90 of the soil passing the geosynthetic
Example of Wet Sieving Apparatus
Tests according to other standards use single grade soil sand or glass-spheres to measure similar properties. Cumulative curve of the granular material passed through the specimen and determination of O 90 cumulative percentage passed (%) sieve opening size (µm) 0 90
Durability Properties Resistance to weathering Resistance to microbiological degradation (soil burial) Resistance to liquids Resistance to hydrolysis Resistance to thermal oxidation
Durability Properties Geosynthetics may be used for temporary structures such as access roads for construction sites or may be required for medium term applications until consolidation of soils makes them redundant. Long-term applications are the main use (30 to 60 years for some in UK application or ; more than 120 years for landfills in most countries). Therefore durability is an important requirement.
Resistance to Weathering (prEN : 1996) Products exposed uncovered to light and products placed without cover- soil for service are tested by artificial weathering. Exposure to UV-light of defined emission spectrum and rain at elevated temperature accelerates the test.
Tensile tests after exposure and reference to fresh specimen tensile strength loss in %. Tensile tests on exposed and fresh specimens can be used to determine the loss of tensile strength, normally expressed as a percentage of strength retained after exposure. Exposure to Natural Weathering
Resistance to Microbiological Degradation (ENV : 1996) Fungi and bacteria living in soils may attack the polymeric materials used as geosynthetics. (There are no recorded failures of geosynthetics due to micro- biological attack). To check the resistance the product to be tested they are buried in biologically active soil and after the soil burial test residual strength is measured. ENV gives types of bacteria and environments be used.
Resistance to Liquids (ENV ISO 12960) The chemical tests developed to date are: the resistance to hydrolysis for Polyester based geosynthetics and the resistance to thermal oxidation for geosynthetics made from Polyolefines.
Immersion of geosynthetics in liquid agents
Resistance to Thermal Oxidation (prEN ISO 13430) To the polyolefine molecules of PE, PP oxygen may be connected creating increased brittleness of the polymers. Stabilizing additives delay this oxidation. For the test the products are exposed to high temperature in an oven.
Resistance to Hydrolysis (pr EN 12447) Hydrolysis of Polyester is the reverse action of the evolution by polycondensation and means connecting water molecules or parts to the PET molecules, thus increasing the Carboxyl end group (CEG)-content and decreasing the average molecular weight often expressed as solution viscosity. External hydrolysis by alkaline attack occurs also at low temperatures, internal hydrolysis in neutral environments is relevant at elevated temperatures. Products are immersed in liquids for times up to 90 days and residual strength and deformation are tested.